Discrete dislocation plasticity analysis of the wedge indentation of films

ARTICLE IN PRESS

Journal **of** **the** Mechanics and Physics **of** Solids

54 (2006) 2281–2303

www.elsevier.com/locate/jmps

**Discrete** **dislocation** **plasticity** **analysis** **of** **the** **wedge**

**indentation** **of** **films**

D.S. Balint a , V.S. Deshpande a, , A. Needleman b , E. Van der Giessen c

a Department **of** Engineering, Cambridge University, Trumpington Street, Cambridge CB2 1PZ, UK

b Division **of** Engineering, Brown University, Providence, RI 02912, USA

c Department **of** Applied Physics, University **of** Groningen, Nyenborgh 4, 9747 AG Groningen, The Ne**the**rlands

Received 2 March 2006; received in revised form 23 June 2006; accepted 3 July 2006

Abstract

The plane strain **indentation** **of** single crystal **films** on a rigid substrate by a rigid **wedge** indenter is

analyzed using discrete **dislocation** **plasticity**. The crystals have three slip systems at 35:3 and 90

with respect to **the** **indentation** direction. The analyses are carried out for three values **of** **the** film

thickness, 2, 10 and 50 mm, and with **the** **dislocation**s all **of** edge character modeled as line

singularities in a linear elastic material. The lattice resistance to **dislocation** motion, **dislocation**

nucleation, **dislocation** interaction with obstacles and **dislocation** annihilation are incorporated

through a set **of** constitutive rules. Over **the** range **of** **indentation** depths considered, **the** **indentation**

pressure for **the** 10 and 50 mm thick **films** decreases with increasing contact size and attains a contact

size-independent value for contact lengths A44 mm. On **the** o**the**r hand, for **the** 2 mm **films**, **the**

**indentation** pressure first decreases with increasing contact size and subsequently increases as **the**

plastic zone reaches **the** rigid substrate. For **the** 10 and 50 mm thick **films** sink-in occurs around **the**

indenter, while pile-up occurs in **the** 2 mm film when **the** plastic zone reaches **the** substrate.

Comparisons are made with predictions obtained from o**the**r formulations: (i) **the** contact sizeindependent

**indentation** pressure is compared with that given by continuum crystal **plasticity**; (ii) **the**

scaling **of** **the** **indentation** pressure with **indentation** depth is compared with **the** relation proposed by

Nix and Gao [1998. Indentation size effects in crystalline materials: a law for strain gradient

**plasticity**. J. Mech. Phys. Solids 43, 411–423]; and (iii) **the** computed contact area is compared with

Corresponding author.

E-mail address: vsd@eng.cam.ac.uk (V.S. Deshpande).

0022-5096/$ - see front matter r 2006 Elsevier Ltd. All rights reserved.

doi:10.1016/j.jmps.2006.07.004

2282

ARTICLE IN PRESS

D.S. Balint et al. / J. Mech. Phys. Solids 54 (2006) 2281–2303

that obtained from **the** estimation procedure **of** Oliver and Pharr [1992. An improved technique for

determining hardness and elastic-modulus using load and displacement sensing **indentation**

experiments, J. Mater. Res. 7, 1564–1583].

r 2006 Elsevier Ltd. All rights reserved.

Keywords: **Discrete** **dislocation**s; Mechanical properties; Size effects; Plasticity; Indentation

1. Introduction

Indentation is used extensively to measure **the** hardness **of** materials. The objective is

usually to draw inferences about **the** mechanical properties (e.g. modulus, yield strength)

**of** **the** material. Tabor (1951) and Johnson (1970) established relationships between

hardness as measured by conical (or pyramidal) and spherical indenters and **the**

stress–strain behavior in **the** regime **of** ‘‘large’’ indents for which conventional **plasticity**

**the**ory is applicable.

When **the** contact area is sufficiently small, in micro- and nano-**indentation**, hardness

values are much increased, giving rise to **the** well-known **indentation** size effect, e.g. Ma

and Clarke (1995), Poole et al. (1996), Swadener et al. (2002), which cannot be accounted

for by conventional **plasticity**. A clear understanding **of** **the** **indentation** size effect and its

connection with material strength is especially important in modern applications involving

thin **films** and multi-layers since nano- and micro-**indentation** are frequently **the** only

means **of** measuring strength, see, for example, Gouldstone et al. (2000) and Lou et al.

(2003). Readers are referred to Freund and Suresh (2004) for fur**the**r details and references.

Simulations based on continuum elastic–plastic analyses have typically been used to

extract **the** plastic properties **of** **the** thin **films** from **the**se nano-**indentation** measurements

(Bhattacharya and Nix, 1988). However, **the**se continuum calculations are unable to

account for **the** size effects typically observed in **the** experiments.

The **indentation** size effect has been one **of** **the** motivations underlying **the** development

**of** a **plasticity** **the**ory for **the** micron scale and **the**re is a large literature concerned with

modeling **indentation** size effects using various non-local **plasticity** **the**ories, e.g. Begley and

Hutchinson (1998), Wei and Hutchinson (2003) and Qu et al. (2006). Nix and Gao (1998)

presented a simple analytical formula for **the** **indentation** size effect based on **the** idea **of**

geometrically necessary **dislocation**s. With **the** characteristic length scale in **the** model used

as a fitting parameter, experimental data have been fit reasonably well, see, for example,

Lou et al. (2003). Similarly, o**the**r modeling frameworks including molecular dynamics

(Horstemeyer et al., 2001), interatomic potential finite element method (Zhu et al., 2003)

and coupled atomistics and discrete **dislocation** **plasticity** (Miller et al., 2004) have also

been used to investigate **the** **indentation** response **of** crystalline solids. However, **the**

‘‘plastic zones’’ in **indentation** problems are sufficiently large that current computational

capabilities restrict **the** molecular dynamics simulations to **the** nano-**indentation** regime.

In principle, discrete **dislocation** **plasticity** should be able to bridge **the** gap between **the**

nano-**indentation** and **the** size-independent continuum regimes. An early three-dimensional

discrete **dislocation** **plasticity** simulation **of** **the** nano-**indentation** **of** copper crystals

was reported by Fivel et al. (1998). While **the**re was good qualitative agreement between

**the** experimentally observed and predicted **dislocation** structures, **the** **indentation** depths in

**the** simulations were too small ð50 nmÞ for **the** **indentation** size effect to be explicitly

ARTICLE IN PRESS

D.S. Balint et al. / J. Mech. Phys. Solids 54 (2006) 2281–2303 2283

investigated. Two-dimensional discrete **dislocation** **plasticity** simulations **of** **indentation**

(Kreuzer and Pippan, 2004, 2005; Polonsky and Keer, 1996) have shown size effects for

both sinusoidal- and **wedge**-shaped indenters. In **the**se simulations, ‘‘low source density’’

materials were considered with **the** **plasticity** size effect mainly resulting from sourcelimited

**plasticity**. Widjaja et al. (2005, 2006) reported on two-dimensional simulations for

**the** cylindrical **indentation** **of** materials with a wide range **of** source densities. Over **the**

range **of** **indentation** depths considered in **the**se studies, **the** increasing hardness with

increasing **indentation** depth associated with sharp indenters was not obtained and **the**

cylinder radius played a dominant role. This is consistent with experimental observations,

see, for example, Swadener et al. (2002).

In previous discrete **dislocation** simulations, **the** **indentation** depths reached were not

sufficiently large to observe **the** transition from a size-dependent hardness to a sizeindependent

‘‘continuum’’ hardness. Here, we consider: (i) **the** effect **of** film thickness on

**indentation** hardness; (ii) **the** scaling **of** **the** hardness in **the** size-dependent regime; and (iii)

**the** transition from a size-dependent to a size-independent hardness. Our study employs

**the** discrete **dislocation** **plasticity** formulation **of** Van der Giessen and Needleman (1995),

which has been extensively used to predict **plasticity** size effects in a variety **of** situations,

including those in bending (Cleveringa et al., 1999) and in **the** uniaxial compression/

tension **of** single crystals (Deshpande et al., 2005).

2. **Discrete** **dislocation** formulation

A plane strain **analysis** **of** **the** **wedge** **indentation** **of** a single crystal film **of** thickness h

and length L rigidly bonded to a rigid substrate is carried out. Plasticity in **the** film is

described by **the** collective motion **of** discrete edge **dislocation**s on specified slip planes.

Complete sticking contact between **the** rigid indenter and **the** film is assumed.

The boundary value problem analyzed is sketched in Fig. 1a. The single crystal film is

elastically isotropic with Young’s modulus E and Poisson’s ratio n, and has three

potentially active slip systems at angles f ðaÞ ða ¼ 1; 2; 3Þ with respect to **the** x 2 -axis.

Plasticity originates from **the** motion **of** edge **dislocation**s, represented as line singularities

in an elastic medium, that can nucleate and glide on **the** active slip planes.

At each stage **of** loading, **the** stress and deformation state is computed using

superposition (Van der Giessen and Needleman, 1995) **of** a singular field and an image

field. The singular field ð~Þ associated with **the** N **dislocation**s is calculated analytically from

**the** isotropic linear elastic **dislocation** fields in a half-space x 2 ph (Freund, 1994). The

complete solution is obtained by adding a smooth image field ð^Þ that ensures that **the**

x 2

ω

A N

h

(a)

elastic/

**dislocation**-free

rigid

L p

L

elastic/

**dislocation**-free

φ (α) x 1

(b)

δ

A

δ s

Fig. 1. (a) Sketch **of** **the** **indentation** boundary value problem analyzed. (b) The definitions **of** **the** actual contact

length A, **the** nominal contact length A N , **the** **indentation** depth d and sink-in d s .

2284

ARTICLE IN PRESS

D.S. Balint et al. / J. Mech. Phys. Solids 54 (2006) 2281–2303

boundary conditions (see Section 2.1 for details) are satisfied. The displacements u i , strains

ij , and stresses s ij are written as

u i ¼ ^u i þ ~u i ; ij ¼ ^ ij þ ~ ij ; s ij ¼ ^s ij þ ~s ij , (1a)

where **the** ð~Þ field is **the** sum **of** **the** fields **of** **the** individual **dislocation**s in **the**ir current

positions, i.e.

~u i ¼ XN

J¼1

~u ðJÞ

i ; ~ ij ¼ XN

J¼1

~ ðJÞ

ij ; ~s ij ¼ XN

J¼1

~s ðJÞ

ij . (1b)

The image field is obtained by solving a linear elastic boundary value problem using finite

elements with **the** boundary conditions changing as **the** **dislocation** structure evolves.

At **the** beginning **of** a calculation, **the** crystal is stress- and **dislocation**-free. The longrange

interactions **of** **the** **dislocation**s are accounted for through **the**ir elastic fields while

constitutive rules are prescribed for short-range interactions. Dislocation dipoles with

Burgers vectors b are nucleated at point sources, that simulate Frank–Read sources,

randomly distributed on discrete slip planes. Nucleation occurs when **the** magnitude **of** **the**

resolved shear stress at **the** source exceeds a critical value t nuc during a time period t nuc . The

sign **of** **the** dipole is determined by **the** sign **of** **the** resolved shear stress along **the** slip plane

while **the** distance between **the** two **dislocation**s at nucleation, L nuc , is taken such that **the**

attractive stress that **the** **dislocation**s exert on each o**the**r is equilibrated by a shear stress **of**

magnitude t nuc . After nucleation, **the** **dislocation**s glide apart, driven by **the** Peach–Koehler

force acting on **the**m, given by

" #

f ðIÞ ¼ m ðIÞ

i

^s ij þ X JaI

~s ðJÞ

ij

þ S ðIÞ

ij

b ðIÞ

j , (2)

where m ðIÞ

i is **the** unit normal to **the** slip system on which **the** **dislocation** with Burgers

vector b ðJÞ

j resides and S ðIÞ

ij is **the** image field on **dislocation** I due to **the** traction-free

surface, i.e. **the** difference between **the** half-space and infinite medium fields. The

magnitude **of** **the** glide velocity V ðIÞ

gln

along **the** slip direction **of** **dislocation** I is taken to be

linearly related to **the** Peach–Koehler force f ðIÞ through **the** drag relation

V ðIÞ

gln ¼ 1 B f ðIÞ , (3)

where B is **the** drag coefficient. Annihilation **of** two oppositely signed **dislocation**s on a slip

plane occurs when **the**y are within a material-dependent critical annihilation distance L e .

Obstacles to **dislocation** motion are modeled as points associated with a slip plane which

pin **dislocation**s that attempt to pass through **the**m. An obstacle releases a pinned

**dislocation** when **the** Peach–Koehler force on **the** obstacle exceeds t obs b, where t obs is **the**

obstacle strength.

2.1. Boundary conditions

Effects **of** geometry changes on **the** momentum balance and lattice rotations are

neglected. However, **the** contact between **the** rigid **wedge** (whose faces are inclined at an

angle o with respect to **the** x 1 -axis) and **the** film is based on **the** deformed film surface. At

**the** current stage **of** deformation, **the** depth **of** **the** **indentation** is denoted by d and **the**

ARTICLE IN PRESS

D.S. Balint et al. / J. Mech. Phys. Solids 54 (2006) 2281–2303 2285

contact length A is defined as **the** range between **the** smallest and **the** largest values **of** x 1

where **the** indenter touches **the** deformed surface. In general, A differs from **the** nominal

contact length A N 2d= tan o due to sink-in or pile-up as sketched in Fig. 1b, but it does

not account for surface roughness which, as shown by Widjaja et al. (2006), can lead to a

significantly smaller contact area in some circumstances and especially for sharp indenters.

Perfect sticking is assumed as soon as **the** **wedge** comes in contact with **the** film so **the** rate

boundary conditions applied are

_u 1 ¼ 0; _u 2 ¼ d _ on S contact , (4a)

where S contact denotes **the** portion **of** **the** deformed surface x 2 ¼ h in contact with **the** **wedge**

and **the** over-dot signifies time differentiation. The o**the**r boundary conditions are

_u 1 ¼ _u 2 ¼ 0; on x 1 ¼L=2 and on x 2 ¼ 0, (4b)

and _T 1 ¼ _T 2 ¼ 0onx 2 ¼ heS contact . Here, T i ¼ s ij n j is **the** surface traction on a surface

with outward normal n j . The applied load is computed as

F ¼

Z L=2

L=2

T 2 ðx 1 ; hÞ dx 1 , (5)

to give **the** **indentation** force versus depth d response. A time step **of** Dt ¼ 0:5 ns is needed

to resolve **the** **dislocation** dynamics. Unless o**the**rwise specified, in order to limit **the**

computation time, a ra**the**r high loading rate _ d ¼ 0:4ms 1 is employed in most **of** **the**

calculations reported below. Some additional calculations at a reduced **indentation** rate **of**

_d ¼ 0:04 ms 1 are also reported.

2.2. Geometry and material properties

Calculations were performed for **films** **of** thickness h ¼ 2, 10 and 50 mm indented by

o ¼ 5 and 10 **wedge**s. These **wedge** angles are smaller than those representative **of**

indenters employed in most experimental studies (e.g. Berkovich or Vickers): larger values

**of** o result in large contact area jumps in **the** discrete **dislocation** calculations and we

restrict this study to op10 . Dislocation activity in a film **of** length L ¼ 1000 mm was

restricted to a process region **of** length L p ¼ 50 mm. The calculations were terminated

before **dislocation**s reached **the** boundaries x 1 ¼L p =2 and thus **the** effect **of** **the** process

region is to restrict **the** **indentation** depths attained in **the** calculations ra**the**r than affect **the**

results presented. The finite element mesh was highly refined in a 30 mm h region around

**the** indenter tip and usually consisted **of** 180 100 bilinear elements with a typical mesh

size **of** about 0:01 mm in a central 1 mm 1 mm region. This ensured that **the** contact was

accurately modeled and that **the** gradients in **the** ð^Þ fields due to **the** **indentation** were

accurately captured.

Unless o**the**rwise specified, **the** crystals have **the** following properties. The film material

has Young’s modulus E ¼ 70 GPa and Poisson’s ratio n ¼ 0:33 and at **the** beginning **of** a

calculation is stress- and **dislocation**-free with slip systems at f ðaÞ ¼35:3 and 90 with

respect to **the** x 2 -axis (this corresponds to **the** slip system orientation in **the** BCC crack

problem in Rice, 1987). Dislocation sources are randomly distributed on slip planes spaced

100b apart, with a density r nuc ¼ 48 mm 2 . Each source is randomly assigned a nucleation

strength t nuc from a Gaussian distribution with average ¯t nuc ¼ 50 MPa and standard

deviation 10 MPa; **the** nucleation time t nuc ¼ 10 ns for all sources. The magnitude **of** **the**

2286

ARTICLE IN PRESS

D.S. Balint et al. / J. Mech. Phys. Solids 54 (2006) 2281–2303

Burgers vector is taken to be b ¼ 0:25 nm for all **dislocation**s. The distance between **the** two

**dislocation**s at nucleation, L nuc , scales with **the** source strength and, on an average, is

L nuc ¼ 0:03 mm. The drag coefficient for **dislocation** motion is B ¼ 10 4 Pa s and **the**

annihilation distance is L e ¼ 6b. Obstacles **of** strength t obs ¼ 150 MPa are randomly

distributed with a density r obs ¼ 98 mm 2 . In addition to this reference crystal, a few

simulations on a crystal with a low density **of** sources and obstacles are also reported.

These low source density (LSD) crystals have r nuc ¼ 9 mm 2 and r obs ¼ 18 mm 2 and all

o**the**r properties **the** same as in **the** reference crystal case.

2.3. Tensile response

The tensile stress–strain responses **of** **the** reference and LSD single crystal materials are

shown in Fig. 2a and b, respectively. These calculations were carried out on tensile bars

having widths w ¼ 1:0–8:0 mm and length L ¼ 3w. As shown in **the** inset **of** Fig. 2a, **the**

three slip systems **of** **the** single crystal are inclined at f ðaÞ ¼35:3 and 90 with respect to

**the** tensile axis, so that **the** tensile response is probed in **the** direction **of** **indentation**. The

computations were performed with an imposed nominal strain rate **of** _¯ ¼ 2000 s 1 ; see

Cleveringa et al. (1999) for details **of** such calculations. The stress–strain behavior is linear

up to a yield strength and **the**n after a transient, **the** overall behavior is essentially nonhardening.

For **the** range **of** specimen sizes considered here, **the** tensile flow strength **of** **the**

reference crystals is approximately independent **of** **the** specimen size, while **the** LSD crystal

shows a noticeable size effect. However, from **the** results in Deshpande et al. (2005), it is

expected that **the** tensile strength **of** **the** reference crystals will eventually increase with

decreasing specimen size. The tensile flow strength ¯s, identified as **the** average stress

between 0:004p¯p0:005 **of** **the** w ¼ 8 mm crystal, is approximately 60 and 50 MPa for **the**

reference and LSD crystals, respectively.

80

w = 1 w = 2

80

w = 1

w = 2

60

60

w = 4

σ (MPa)

40

w = 8

w = 4

σ (MPa)

40

w = 8

20

φ (α)

20

U

U w

(a)

0

0

L

0

0.001 0.002 0.003 0.004 0.005

0 0.001 0.002 0.003 0.004 0.005

ε

(b)

ε

Fig. 2. The tensile stress versus strain response **of** **the** (a) reference (r src ¼ 48 mm 2 , r obs ¼ 98 mm 2 ) and (b) low

source density (r src ¼ 9 mm 2 , r obs ¼ 18 mm 2 ) crystals. The responses are shown for four selected specimen sizes

w (dimensions in mm) in each case and **the** tensile boundary value problem is as sketched in **the** inset in (a).

ARTICLE IN PRESS

D.S. Balint et al. / J. Mech. Phys. Solids 54 (2006) 2281–2303 2287

0.03

0.025

elastic/plastic

elastic

h = 2µm

0.03

0.025

F (N µm -1 )

0.02

0.015

0.01

h = 10µm

F (N µm -1 )

0.02

0.015

0.01

h = 2µm

h = 10µm

0.005

0.005

0

0

(a)

0

0.1 0.2 0.3 0.4

0 0.1 0.2 0.3 0.4

δ (µm)

(b)

δ (µm)

Fig. 3. Indentation force versus applied **indentation** depth for **the** (a) o ¼ 5 and (b) o ¼ 10 **wedge**s. Results are

shown for two selected film thicknesses h and both **the** elastic and discrete **dislocation** predictions for **the** reference

material are included.

3. Indentation response **of** **the** reference crystal **films**

The **indentation** force F versus applied **indentation** depth d response **of** **the** h ¼ 2 and

10 mm **films** is plotted in Fig. 3a and b for **the** o ¼ 5 and 10 indenters, respectively.

Predictions for elastic **films** (i.e. without any **dislocation** activity) are also included for

reference purposes. The **indentation** force increases approximately quadratically with

displacement in all cases. For a given **indentation** depth, **the** **indentation** force increases

with decreasing film thickness and increasing **wedge** angle o. A comparison with **the**

**indentation** forces for **the** purely elastic film reveals that **the** **plasticity** caused by **the**

**dislocation** activity significantly relaxes **the** stresses in **the** **films**, thus reducing **the**

**indentation** force.

The variation **of** **the** actual contact length 1 A with **the** applied displacement d is plotted in

Fig. 4a and b for **the** o ¼ 5 and 10 **wedge**s, respectively. Results are included in Fig. 4 for

all three film thicknesses. For reference purposes, **the** variation **of** **the** nominal contact

length, A N 2d= tan o, with displacement is also included in Fig. 4. There are large jumps

(much larger than **the** finite element mesh size) in **the** contact length. These jumps occur

because material sink-in results in a portion **of** **the** deformed film surface outside **the** contact

length becoming nearly parallel to **the** surface **of** **the** **wedge** indenter. Thus, continued

**indentation** results in **the** contact length increasing in bursts (**the** spikes in **the** force versus

displacement curves in Fig. 3 correspond to **the**se jumps in **the** contact length). The

prediction **of** **the** A versus d relation for a second realization **of** sources and obstacles (same

initial densities as **the** reference case) is included in Fig. 4b for **the** h ¼ 10 mm film indented by

**the** o ¼ 10 **wedge**. It is clear from a comparison **of** **the** predictions for **the** two realizations

that while **the** general trends are similar for both realizations, **the** jumps are stochastic in

nature and depend on **the** details **of** **the** initial source and obstacle distributions.

1 What is termed **the** actual contact length here is referred to as **the** end-to-end contact length in Widjaja et al.

(2006).

2288

ARTICLE IN PRESS

D.S. Balint et al. / J. Mech. Phys. Solids 54 (2006) 2281–2303

14

12

A N

h = 2 µm

6

5

A N

h = 2 µm

A (µm)

10

8

6

4

h = 50 µm

A (µm)

4

3

2

h = 50 µm

2

0

h = 10 µm

1

0

h = 10µm

(a)

0

0.1 0.2 0.3 0.4 0 0.1 0.2 0.3 0.4

δ (µm)

(b)

δ (µm)

Fig. 4. The relation between **the** actual contact length A and **indentation** depth d for **indentation** **of** **the** reference

material with **the** (a) o ¼ 5 and (b) o ¼ 10 **wedge**s. Results are shown for three film thicknesses h. The

prediction for a second realization **of** **the** reference material is included in (b) for **the** h ¼ 10 mm film (dotted curve).

Fig. 5. The deformed mesh (displacements magnified by a factor **of** 2) in **the** o ¼ 10 **wedge** **indentation** **of** **the**

(a) h ¼ 2 mm and (b) h ¼ 50 mm **films** **of** **the** reference material. The meshes are shown at **the** instant when **the**

actual contact length A ¼ 4 mm.

The actual contact length A is less than **the** nominal contact length for **the** h ¼ 10 and

50 mm **films** (especially so for **the** o ¼ 10 indenter) while A4A N for **the** h ¼ 2 mm **films** at

**indentation** depths greater than 0:1 and 0:2 mm for **the** o ¼ 5 and 10 indenters,

respectively. This is a result **of** material pile-up for **the** h ¼ 2 mm film and sink-in for **the**

thicker **films**. To illustrate this, deformed meshes for **the** o ¼ 10 **indentation** **of** **the** h ¼ 2

and 50 mm **films** are shown in Fig. 5a and b, respectively, at **the** instant when **the** actual

contact length A ¼ 4 mm. These figures show material pile-up for **the** 2 mm film and sink-in

for **the** 50 mm film. However, it is worth noting that material sink-in occurs for small

**indentation** depths even in **the** h ¼ 2 mm **films** (resulting in AoA N , see Fig. 4) and pile-up

begins when **the** plastic zone under **the** indenter reaches **the** rigid substrate at x 2 ¼ 0. Pileup

may eventually occur in **the** 10 and 50 mm **films**, albeit at much larger **indentation**

depths than considered here. In order to explore **the** effect **of** **the** side constraint in Eq. (4b)

on **the** evolution **of** pile-up, calculations were carried out with traction-free boundary

conditions on x 1 ¼L=2. This change in boundary conditions had no effect on **the**

development **of** pile-up, indicating that material pile-up does result from **the** plastic zone

extending to **the** bottom surface **of** **the** film, x 2 ¼ 0, and is not a consequence **of** **the** side

constraint.

ARTICLE IN PRESS

D.S. Balint et al. / J. Mech. Phys. Solids 54 (2006) 2281–2303 2289

1500

1500

1200

h = 2 µm

1200

h = 2 µm

p (MPa)

900

600

300

p/5,

h = 10 µm elastic, h = 50 µm

p (MPa)

900

h = 10 µm

600

300

(a)

0

continuum (τ 0 = 50 MPa) h = 50µm

0 2 4 6 8

A (µm)

(b)

continuum ( τ 0 = 50 MPa) h = 50 µm

0

0 1 2 3 4 5

A (µm)

Fig. 6. The **indentation** pressure p versus actual contact length A relation for **indentation** **of** **the** reference material

with **the** (a) o ¼ 5 and (b) o ¼ 10 **wedge**s. Results are shown for three film thicknesses h. The continuum

predictions **of** **the** nominal **indentation** pressure for a large crystal are also included. In addition, **the** **indentation**

pressure for an elastic material is also shown in (a) with p divided by five to fit **the** scale.

The **indentation** pressure p is defined as **the** ratio **of** **the** **indentation** force and **the** actual

contact length, viz.

p ¼ F A . (6)

The **indentation** pressure versus actual contact length relation is plotted in Fig. 6a and b

for **the** o ¼ 5 and 10 indenters, respectively. The **indentation** pressure versus contact

length relation for **the** elastic h ¼ 50 mm film indented by **the** o ¼ 5 **wedge** is also included

in Fig. 6a. No length scale exists in **the** elastic problem (over **the** **indentation** depths

considered here) and thus we expect no size effect in **the** elastic problem. The numerical

simulations correctly predict this size independence for A40:05 mm: for smaller contact

lengths, **the** numerical length scale introduced by **the** finite element discretization affects

**the** results. Convergence studies carried out to determine **the** effect **of** **the** numerical length

scale introduced by **the** finite element discretization on **the** elastic–plastic results revealed

that fur**the**r mesh refinement only affected **the** results for contact depths **of** four to five

times **the** element length (i.e. d 0:05 mm). These data are excluded from Fig. 6 and **the**

elastic–plastic results presented in Fig. 6 are over **the** range where **the** simulations are

essentially mesh size-independent.

The results in Fig. 6 show that **the** **indentation** pressure decreases with increasing contact

length, before leveling **of**f in **the** h ¼ 10 and 50 mm **films** at p 300 MPa for contact lengths

A44 mm. The **indentation** pressure versus contact length relations for **the** h ¼ 10 and

50 mm **films** are almost identical. 2 Bouvier and Needleman (2006) recently reported

continuum crystal **plasticity** calculations for **wedge** **indentation** **of** single crystals and we

repeated **the**ir calculations for **the** crystallographic orientation and **wedge** geometries used

2 The differences between **the** h ¼ 10 and 50 mm responses in Fig. 6b are a result **of** jumps in **the** actual contact

length which to a large extent are stochastic in nature. However, **the** **indentation** force versus **indentation** depth

curves for **the**se two cases are almost identical.

2290

ARTICLE IN PRESS

D.S. Balint et al. / J. Mech. Phys. Solids 54 (2006) 2281–2303

here with a slip system flow strength t 0 ¼ 50 MPa and no material hardening. The nominal

**indentation** pressures predicted by **the** continuum crystal **plasticity** calculations are

included in Fig. 6. The discrete **dislocation** predictions asymptote towards **the** continuum

crystal **plasticity** **indentation** pressure limits that are size-independent.

The differences between **the** continuum and discrete **dislocation** predictions are fur**the**r

highlighted by comparing **the** distributions **of** **the** quantity

G ¼ X3

jg ðaÞ j,

a¼1

where g ðaÞ is given by

(7a)

Here, s ðaÞ

i

g ðaÞ ¼ s ðaÞ

i ij m ðaÞ

j . (7b)

and m ðaÞ

j are unit vectors tangential and normal, respectively, to slip system a.

Since **dislocation** glide gives rise to a displacement jump across **the** slip plane, **the**

displacement field is not continuous. In order to visualize **the** deformation, we evaluate G

in **the** discrete **dislocation** simulations by evaluating **the** displacements u i on a uniform grid

with cell size 0:25 mm. The strain field ij is **the**n obtained by numerical differentiation using

bilinear displacement shape functions. Although it is convenient to use G for picturing **the**

deformation mode, G in Fig. 7a is not a direct measure **of** slip since g ðaÞ is not **the** actual slip

on slip plane a as it includes contributions from **dislocation**s gliding on all slip systems. On

**the** o**the**r hand, for continuum crystal **plasticity**, Fig. 7b, g ðaÞ ¼ s ðaÞ

i p ij mðaÞ j , where p ij is **the**

plastic strain.

Distributions **of** G at an **indentation** depth d ¼ 0:4 mm in **the** h ¼ 50 mm film (o ¼ 5 ) are

plotted in Fig. 7a and b using **the** discrete **dislocation** and continuum crystal **plasticity**

constitutive descriptions, respectively. The values **of** G in Fig. 7a give a measure **of** slip

averaged over approximately 10 slip planes (**the** grid size used to evaluate strain is 0:25 mm

while **the** slip plane spacing in **the** discrete **dislocation** simulations is 0:025 mm). The

discrete **dislocation** **plasticity** results give a larger ‘‘plastic’’ zone than **the** continuum

Γ

0 0.04 0.08 0.12

Γ

0 0.04 0.08 0.12

(a)

30 µm

(b)

30 µm

Fig. 7. Distribution **of** **the** total slip G in **the** h ¼ 50 mm film indented by **the** o ¼ 5 **wedge** indenter to an

**indentation** depth d ¼ 0:4 mm (A ¼ 7:5 mm). (a) **Discrete** **dislocation** prediction for **the** reference material and (b)

continuum crystal **plasticity** prediction for a crystal with a slip system strength t 0 ¼ 50 MPa. The distributions are

shown on **the** deformed film (no magnification **of** **the** deformation).

ARTICLE IN PRESS

D.S. Balint et al. / J. Mech. Phys. Solids 54 (2006) 2281–2303 2291

crystal **plasticity** calculations. In particular, **plasticity** occurs only under **the** indenter in **the**

continuum calculations. In **the** discrete **dislocation** calculations, slip emanates on **the** f ¼

35:3 slip planes from **the** edge **of** **the** contact, and thus **the** plastic zone spreads outside

**the** contact region.

The discrete **dislocation** calculations **of** **the** 50 mm film predict that **the** **indentation**

pressure p decreases with increasing contact length (Fig. 6) for contact lengths less than

about 4 mm. This **indentation** size effect has typically been attributed to geometrically

necessary **dislocation**s. The **dislocation** distributions at **indentation** depths d ¼ 0:2 and

0:4 mm for **the** o ¼ 5 **wedge** **indentation** **of** **the** h ¼ 50 mm film are plotted in Fig. 8a and b,

respectively. These **dislocation** distributions differ from what is assumed in an idealized

model such as that **of** Nix and Gao (1998). One contribution to this difference is that **the**

discrete **dislocation** calculations give rise to both statistically stored and geometrically

necessary **dislocation**s, but **the**re is also a difference in **the** number and orientation **of** **the**

slip systems.

The results for **the** h ¼ 2 mm film are qualitatively different over **the** range **of** **indentation**

depths considered here. For both **the** o ¼ 5 and 10 indenters, **the** **indentation** pressure

decreases with increasing contact length for Ao2 mm (corresponding to d 0:1 and 0:2 mm

for **the** o ¼ 5 and 10 indenters, respectively). Subsequently, when **the** plastic zone

reaches **the** substrate x 2 ¼ 0, **the** **indentation** pressure increases with increasing contact

length and no contact size-independent limit is reached. The discrete **dislocation** results

indicate that **the** **indentation** pressure increases with increasing **indentation** depth for

d=h40:05 and 0.1 for **the** o ¼ 5 and 10 **wedge**s, respectively. While **the** calculated

**indentation** depths at which an increase in **indentation** pressure occurs are comparable to

those seen experimentally by Han et al. (2006) and Saha et al. (2001), a quantitative

comparison is not appropriate because **the** situation modeled here differs from that in **the**

experiments in a variety **of** ways including differences in **the** indenter geometry and in **the**

Fig. 8. The **dislocation** structure in a central 20 mm 20 mm region around **the** indenter tip in **the** h ¼ 50 mm film

**of** **the** reference material indented to (a) d ¼ 0:2 mm and (b) d ¼ 0:4 mm by **the** o ¼ 5 **wedge**.

2292

ARTICLE IN PRESS

D.S. Balint et al. / J. Mech. Phys. Solids 54 (2006) 2281–2303

elastic mismatch between **the** film and **the** substrate. Saha et al. (2001) have shown that

appropriately calibrated strain gradient **plasticity** **the**ories are capable **of** predicting this

initial decrease and **the**n increase in hardness with increasing **indentation** depth for **the** thin

**films**, while conventional **plasticity** calculations significantly over-predict **the** **indentation**

depths at which **the** plastic zone interacts with **the** substrate.

The variation **of** **the** nominal **indentation** pressure p N F=A N with nominal contact

length A N is plotted in Fig. 9a and b for **the** o ¼ 5 and 10 **wedge**s, respectively. A

comparison with Fig. 6 reveals that **the** nominal **indentation** pressure p N op in **the** early

stages **of** **the** **indentation**, especially for **the** o ¼ 10 **wedge**s. The trend reverses at large

**indentation** depths for **the** h ¼ 2 mm film when pile-up results in **the** actual contact length

exceeding **the** nominal contact length. The discrete **dislocation** **plasticity** predictions **of** **the**

p N versus A N relation for **indentation** **of** **the** h ¼ 50 mm **films** at _ d ¼ 0:04 ms 1 are also

included in Fig. 9. The nominal **indentation** pressure at **the** lower **indentation** rate is about

25% less than that at **the** reference **indentation** rate at small contact lengths. However, this

difference is reduced to only about 5% lower at large contact lengths where **the** **indentation**

pressure is essentially size independent.

The distribution **of** **the** stress s 22 under **the** o ¼ 5 indenter in **the** h ¼ 2 and 50 mm **films**

is plotted in Fig. 10a and b, respectively. These plots correspond to an **indentation** depth

d ¼ 0:4 mm and actual contact lengths A 12 and 8 mm for **the** h ¼ 2and50mm **films**,

respectively. In Fig. 10a, high compressive stresses are seen to develop beneath **the** contact

zone while a tensile stress s 22 is generated at **the** edges **of** **the** contact zone. The stress

distribution in **the** h ¼ 2 mm film is clearly affected by **the** rigid substrate and is

qualitatively different from **the** distribution in **the** h ¼ 50 mm film.

We define **the** lattice rotation O as

O ¼ 1 2 ð ^u 2;1 þ ~u 2;1 ^u 1;2 ~u 1;2 Þ, (8)

1500

1200

δ=0.4 ms -1

δ=0.04 ms -1

1500

1200

δ=0.4 ms -1

δ=0.04 ms -1

p N (MPa)

900

600

h = 2 µm

p N (MPa)

900

600

h = 2 µm

(a)

300

0

h = 10 µm

h = 50 µm continuum (τ 0 = 50 MPa)

0 2 4 6 8

A N (µm)

(b)

300

0

h = 10 µm

h = 50 µm

continuum (τ 0 = 50 MPa)

0 1 2 3 4 5

A N (µm)

Fig. 9. The nominal **indentation** pressures p N versus nominal contact length A N for **indentation** **of** **the** reference

material with **the** (a) o ¼ 5 and (b) o ¼ 10 **wedge**s. Results are shown for three film thicknesses h. The

continuum predictions **of** **the** nominal **indentation** pressures for a large crystal are also included.

ARTICLE IN PRESS

D.S. Balint et al. / J. Mech. Phys. Solids 54 (2006) 2281–2303 2293

Fig. 10. The distribution **of** **the** stress s 22 in **the** (a) h ¼ 2 mm and (b) h ¼ 50 mm **films** **of** **the** reference material

indented to d ¼ 0:4 mm by **the** o ¼ 5 **wedge**. The distributions are shown on **the** deformed film (no magnification

**of** **the** deformation).

Ω (degrees)

-1.44 -0.72 0 0.72 1.44

20 µm

20 µm

(a)

20 µm

(b)

20 µm

Fig. 11. The distribution **of** **the** lattice rotations under **the** indenter in **the** h ¼ 50 mm film **of** **the** reference material

indented to d ¼ 0:4 mm by **the** (a) o ¼ 5 and (b) o ¼ 10 **wedge**s. The distribution is shown in a central 20 mm

20 mm region around **the** indenter tip in **the** deformed film (no magnification **of** **the** deformation).

where **the** spatial differentiation ~u i;j is performed analytically to exclude **the** slip

contribution **of** **the** ð~Þ fields. Contours **of** **the** lattice rotation O at d ¼ 0:4 mm are plotted

in Fig. 11a and b for **indentation** **of** **the** h ¼ 50 mm film by **the** o ¼ 5 and 10 indenters,

respectively. As in **the** recent experimental results **of** Kysar et al. (2005) for o ¼ 45 **wedge**

**indentation** **of** copper single crystals, **the**re is a ra**the**r abrupt change in **the** sign **of** **the**

lattice rotation on **the** line x 1 ¼ 0 immediately below **the** indenter. The continuum crystal

2294

ARTICLE IN PRESS

D.S. Balint et al. / J. Mech. Phys. Solids 54 (2006) 2281–2303

**plasticity** simulations **of** Bouvier and Needleman (2006), which assume symmetry about

x 1 ¼ 0, also predict a reasonably abrupt change in **the** sign **of** **the** lattice orientation.

4. Effect **of** source and obstacle density

In **the** **indentation** size effect observed in **the** results presented in Section 3 both strain

gradients (and **the** consequent generation **of** geometrically necessary **dislocation**s) imposed

by **the** **indentation** process and source-limited **plasticity** (i.e. no available **dislocation**

sources at locations **of** high stress) likely come into play. To explore **the** relative role **of**

limited **dislocation** sources, we analyze **indentation** **of** a crystal with a lower density **of**

**dislocation** sources.

The predicted **indentation** pressure p versus actual contact length A relation for **the**

o ¼ 5 **indentation** **of** **the** h ¼ 10 and 50 mm **films** **of** **the** LSD material (r src ¼ 9 mm 2 ,

r obs ¼ 18 mm 2 ) is plotted in Fig. 12a. For comparison purposes, **the** corresponding results

for **the** reference material (Fig. 6a) are also included. The **indentation** pressure is higher for

**the** LSD crystal over **the** range **of** contact lengths considered here. While a contact sizeindependent

**indentation** pressure was achieved for A44 mm in **the** reference material, a

contact size-independent limit was not attained in **the** LSD material until A48 mm.

However, it does appear that **the** LSD and reference material responses converge to **the**

same limit at large contact lengths. A comparison between **the** contact length A versus

**indentation** depth d relation for **the** h ¼ 10 and 50 mm **films** with **the** reference and LSD

crystal properties is shown in Fig. 12b. The reduced **plasticity** in **the** LSD material results

in increased material sink-in, though as for **the** **indentation** pressure results, **the** LSD and

reference material curves appear to converge for large **indentation** depths. Although

qualitatively **the** size-dependence **of** **the** reference and LSD crystals is similar, for a given

**indentation** depth **the** **indentation** pressure **of** **the** LSD crystal is significantly greater than

1500

1200

LSD

reference crystal

10

8

LSD

reference crystal

A N

p (MPa)

900

600

300

h = 10 µm

A (µm)

6

4

2

h = 10 µm

h = 50 µm

(a)

0

continuum (τ 0 = 50 MPa) h = 50 µm

0 2 4 6 8

A (µm)

(b)

0

0

0.1 0.2 0.3 0.4

A (µm)

Fig. 12. A comparison between **the** o ¼ 5 **indentation** **of** **the** reference (r src ¼ 48 mm 2 , r obs ¼ 98 mm 2 ) and

LSD (r src ¼ 9 mm 2 , r obs ¼ 18 mm 2 ) **films**. (a) Actual **indentation** pressure versus actual contact length and

(b) actual contact length as a function **of** **indentation** depth. Results are shown for **the** h ¼ 10 and 50 mm **films**.

ARTICLE IN PRESS

D.S. Balint et al. / J. Mech. Phys. Solids 54 (2006) 2281–2303 2295

that **of** **the** reference crystal. Thus, limited **dislocation** sources can provide a significant

contribution to **the** **indentation** pressure at small **indentation** depths.

5. Comparison with **the** Nix–Gao model

Nix and Gao (1998) developed a model to capture **the** variation **of** **the** **indentation**

pressure with **indentation** depth based on **the** role **of** geometrically necessary **dislocation**s.

They first calculated **the** density **of** geometrically necessary **dislocation**s from geometric

arguments and **the**n employed **the** Taylor relation for **the** scaling **of** strength with

**dislocation** density to derive **the** **indentation** pressure versus **indentation** depth relation as

rffiffiffiffiffiffiffiffiffiffiffiffiffi

p

¼ 1 þ d

. (9)

p 0 d

Here, d is a characteristic length that depends on **the** **wedge** angle and p 0 is **the** **indentation**

pressure in **the** infinite **indentation** depth limit. We note that in **the** Nix–Gao model nei**the**r

p 0 nor d p

are intrinsic material properties with p 0 / ffiffiffiffi r s,

where rs is **the** density **of**

statistically stored **dislocation**s while **the** characteristic length d depends on **the**

statistically stored **dislocation** density through p 0 via **the** scaling relation d / p0 2.

The discrete **dislocation** **plasticity** predictions **of** **the** **indentation** pressure p versus

**indentation** depth d relation for **the** reference crystal indented by **the** o ¼ 5 **wedge** is

plotted in Fig. 13 for **the** three film thicknesses considered. We observe that **the** **indentation**

pressure drops sharply at d 0:1 mm. For **the** two thicker **films**, **the** **indentation** pressure

**the**n decreases smoothly with increasing d before leveling **of**f at d 0:4 mm. The very high

**indentation** pressures at do0:1 mm are a result **of** **the** fact that **the** actual contact length

remains nearly unchanged in **the** range 0pdp0:1 mm (Fig. 4a). It is clear from Fig. 13 that

Eq. (9) will not provide a good fit to **the** discrete **dislocation** predictions **of** **the** actual

**indentation** pressure versus d relation.

1600

1200

h = 2 µm

p (MPa)

800

400

h = 10 µm

0

0

continuum (τ 0 = 50 MPa)

0.1 0.2

δ (µm)

h = 50 µm

0.3

0.4

Fig. 13. **Discrete** **dislocation** predictions **of** **the** **indentation** pressure p versus **indentation** depth d relation **of** **the**

reference material. Results are shown for three selected film thicknesses h.

2296

ARTICLE IN PRESS

D.S. Balint et al. / J. Mech. Phys. Solids 54 (2006) 2281–2303

However, we proceed to demonstrate that **the** discrete **dislocation** predictions **of** **the**

nominal **indentation** pressure versus **indentation** depth are reasonably well represented by

**the** Nix and Gao (1998) relation. The nominal **indentation** pressure versus **indentation**

depth predictions for **the** o ¼ 5 and 10 **wedge** **indentation** **of** **the** h ¼ 50 mm **films** **of** **the**

reference material are plotted in Fig. 14a. The best fits to **the** discrete **dislocation**

predictions using **the** relation Eq. (9) (with p 0 and d as free parameters given by a leastsquares

fit) are included in Fig. 14a, with **the** values **of** **the** parameters listed in Table 1.

Note that Eq. (9) is fit to **the** ‘‘plastic’’ part **of** **the** p N versus d curve and **the**n backextrapolated

to **the** smaller **indentation** depths as shown in Fig. 14a. The Nix and Gao

(1998) relation fits **the** discrete **dislocation** predictions reasonably well. However, **the** bestfit

parameters for **the** o ¼ 10 indenter have a value **of** p 0 much lower than **the** value given

by a continuum **plasticity** calculation. Moreover, **the** value obtained for **the** material length

scale d is 4:9 mm: this is much larger than **the** slip plane spacing or **the** **dislocation** source

and obstacle spacings and is not clearly related to any physical material length scale **of** **the**

reference material.

1500

1200

DD prediction

fit **of** form (9)

extrapolation **of** fit

800

600

ω = 5°

DD prediction

fit **of** form (9)

p N (MPa)

900

600

p N (MPa)

400

LSD crystal

(a)

300

0

0

ω = 10°

200

reference crystal

ω = 5°

0

0.1 0.2 0.3 0.4

0 0.1 0.2 0.3 0.4

δ (m)

(b)

δ (m)

Fig. 14. Comparisons between **the** discrete **dislocation** predictions for **the** **indentation** **of** **the** h ¼ 50 mm **films** and

best fits **of** **the** Nix–Gao relation Eq. (9) (**the** parameter values are given in Table 1) for (a) **the** o ¼ 5 and 10

**indentation** **of** **the** reference crystals and (b) **the** o ¼ 5 **indentation** **of** **the** LSD and reference crystals.

Table 1

The parameters used to plot Eq. (9) in Fig. 14

Material Wedge angle o (deg.) Parameters for Eq. (9) Parameters for Eq. (10)

p 0 (MPa) d ðmmÞ p 0 (MPa) d ðmmÞ n

Reference 5 142 0.28 163 0.10 0.70

Reference 10 61 4.9 107 0.84 0.64

LSD 5 47 6.7 131 0.37 0.68

The best-fit parameters for Eq. (10) are also included.

ARTICLE IN PRESS

D.S. Balint et al. / J. Mech. Phys. Solids 54 (2006) 2281–2303 2297

In order to determine whe**the**r a power-law exponent o**the**r than 0.5 gives a more

appropriate fit to **the** discrete **dislocation** results, we consider a relation **of** **the** form

p n

N

¼ 1 þ d

. (10)

p 0 d

Using **the** parameters listed in Table 1, this relation gives fits nearly identical to those

shown in Fig. 14a. Interestingly, with power-law exponents n 0:65–0:7 **the** best-fit value

for p 0 is closer to **the** continuum crystal **plasticity** prediction than when n is fixed at 0:5 and

d is **of** **the** order **of** **the** source and obstacle spacings in **the** material.

The nominal **indentation** pressure versus **indentation** depth predictions for **the** o ¼ 5

**wedge** **indentation** **of** **the** h ¼ 50 mm **films** with **the** reference as well as with **the** LSD crystal

properties are plotted in Fig. 14b along with **the** best fits **of** Eq. (9) (**the** fitting parameters

are listed in Table 1). The best-fit parameters for **the** LSD material using Eq. (10) are also

listed in Table 1. For **the** LSD crystals with n40:5, **the** parameter p 0 also has a value that is

representative **of** its large **indentation** depth value and d has a greater value than for **the**

reference material, indicating that d increases with **the** average **dislocation** source and

obstacle spacings.

The linear dependence **of** **the** square **of** **the** **indentation** pressure ðp=p 0 Þ 2 with **the** inverse

**indentation** depth 1=d as predicted by Nix and Gao (1998) is in good agreement with a

wide body **of** experimental evidence for **indentation** depths d41 mm. But **the** fit over a

wider range **of** **indentation** depths is not as good; see, for example, Poole et al. (1996),

Gerberich et al. (2002) and Swadener et al. (2002). This is consistent with **the** conical

**indentation** simulations **of** Begley and Hutchinson (1998) using **the** Fleck and Hutchinson

(1997) strain gradient **plasticity** **the**ory which do not predict **the** Nix and Gao (1998)-type

scaling over **the** full range **of** **indentation** depths. Begley and Hutchinson (1998) suggested

that alternative descriptions **of** **the** effective strain (which governs **the** interaction between

**the** statistical and geometrically necessary **dislocation**s) in **the** Fleck and Hutchinson (1997)

strain gradient **plasticity** model could be employed to obtain **the** Nix and Gao (1998)-type

scaling. Recently, Abu Al-Rub and Voyiadjis (2004) have proposed a form **of** **the** effective

strain relation in **the** Fleck and Hutchinson (1997) model that does indeed reproduce **the**

Nix and Gao (1998) scaling relation. Huang et al. (2006) have proposed an extension **of** **the**

Nix–Gao model based on **the** assumption that **the**re exists a maximum allowable density **of**

geometrically necessary **dislocation**s.

The discrete **dislocation** results suggest that exponents in **the** range 0.6–0.7, ra**the**r than 0.5

as in Eq. (9), are more suitable for describing **the** **indentation** size effect in **the** present

calculations. There are several possible reasons for this including: (i) **the** current twodimensional

discrete **dislocation** **plasticity** simulations do not give rise to **the** square root

Taylor relation on which Eq. (9) is based, although this can be included by using **the**

extended set **of** constitutive rules suggested by Benzerga et al. (2004); (ii) **the** **indentation**

depths in **the** calculations presented here are restricted to dp0:4 mm and, as discussed by

Abu Al-Rub and Voyiadjis (2004), **the** Nix and Gao (1998) model is most appropriate for

**indentation** depths d41 mm; (iii) **the** models **of** Nix and Gao (1998) and **of** Huang et al.

(2006) essentially assume no interaction between **the** statistically stored and geometrically

necessary **dislocation**s and this interaction occurs naturally in **the** discrete **dislocation**

**plasticity** calculations; (iv) **the** Nix and Gao (1998) and Huang et al. (2006) models assume a

hemispherical plastic zone with a radius equal to **the** nominal contact radius and **the** single

crystal discrete **dislocation** calculations (see Fig. 7a) give a much larger plastic zone size; and

2298

ARTICLE IN PRESS

D.S. Balint et al. / J. Mech. Phys. Solids 54 (2006) 2281–2303

(v) **the** calculations here are carried out for **wedge** angles o smaller than representative **of**

typical indenters used in **the** experiments and **the** discrete **dislocation** calculations suggest

that **the** best-fit exponent n decreases somewhat with increasing **wedge** angle.

6. Estimation **of** **the** contact area

Experimentally, measuring **the** true contact area is difficult, if not impossible. To avoid

**the** need for **the** determination **of** true contact area, **the** hardness is sometimes identified

with **the** nominal **indentation** pressure p N , ra**the**r than true **indentation** pressure (Ma and

Clarke, 1995; Poole et al., 1996). The results here (see Figs. 6 and 9) indicate that sink-in

occurs in **the** size regime where **the**re is a significant size-dependent increase in hardness.

Hence, **the** **indentation** size effect **of** **the** increasing **indentation** pressure with decreasing

contact size might be even more significant than that suggested by **the** experiments as sinkin

during **the** early stages **of** **the** **indentation** results in **the** actual contact length being less

than **the** nominal contact length. In o**the**r circumstances, an unloading procedure

suggested by Oliver and Pharr (1992) (also see Oliver and Pharr (2004) for a review **of**

various refinements to **the** original method) is used which is based on **the** assumption that

**the** sink-in can be modeled by elastic **indentation** **of** a half-space by a rigid punch having a

simple geometry. In particular, **the** sink-in d s (see Fig. 1b) at an **indentation** load F max is

given by (Oliver and Pharr, 1992)

d s ¼ Z F max

S , (11)

where S dF=ddj F¼F max

is **the** initial slope **of** **the** unloading curve from F max and Z is a

non-dimensional constant that depends on **the** geometry **of** **the** indenter and **the** film

thickness. The procedure **the**n is to determine **the** initial unloading stiffness S from

experimental measurements, extract d s from Eq. (11) and estimate **the** actual contact length

A at **the** **indentation** load F max via **the** geometrical relation

A ¼ 2ðd max d s Þ

. (12)

tan o

The procedure **of** Oliver and Pharr (1992) has been shown to hold for **the** **indentation** **of**

solids modeled by conventional isotropic continuum **plasticity**, see, for example, Cheng

and Cheng (1997). Here, we explore **the** extent to which this procedure can estimate **the**

actual contact length A in **the** discrete **dislocation** **plasticity** **indentation** calculations.

Fig. 15a shows **the** unloading response from six **indentation** depths in **the** h ¼ 50 mm film

with **the** reference crystal properties for **the** o ¼ 5 indenter. The predictions for **the** initial

unloading response from six selected values **of** **the** **indentation** force are also included in

Fig. 15a. These unloading simulations were carried out at an unloading rate d _ ¼ 0:4ms 1

with nodes stuck to **the** rigid indenter released from **the** contact when **the** inter-facial

traction T 2 becomes tensile. The initial unloading stiffness S is estimated from **the**se

calculations and **the** discrete **dislocation** **plasticity** predictions **of** **the** variation **of** **the** sinkin

d s (calculated from Eq. (12) as **the** actual contact area A is known directly from **the**

simulation) at F ¼ F max with F max =S is plotted in Fig. 15b. Here, F max is **the** **indentation**

load at **the** onset **of** unloading. In addition, **the** prediction **of** **the** d s versus F max =S relation

from an elastic calculation **of** **the** o ¼ 5 **wedge** **indentation** **of** **the** h ¼ 50 mm film is also

included in Fig. 15b and **the**se finite element calculations suggest that **the** proportionality

ARTICLE IN PRESS

D.S. Balint et al. / J. Mech. Phys. Solids 54 (2006) 2281–2303 2299

0.002

0.0015

simulation

fit to unloading data

VI

0.1

0.08

S from simulation

S from fit to unloading data

F (N µm -1 )

0.001

0.0005

I

III

II

IV

V

δ s (µm)

0.06

0.04

0.02

I

IV

II

III

V

VI

IV V

VI III

elastic calculation

(a)

0

0

0.1 0.2 0.3 0.4

δ (µm)

(b)

0

0

0.01

0.02 0.03 0.04

F max / S (µm)

0.05

Fig. 15. (a) The loading and unloading **indentation** force versus depth predictions for **the** h ¼ 50 mm film by **the**

o ¼ 5 indenter and (b) **the** variation **of** **the** sink-in depth d s with **the** initial unloading stiffness S.

Table 2

The parameters used to fit Eq. (13) to **the** unloading discrete **dislocation** predictions in Fig. 15a

Unloading curve a m Correlation coefficient, R

N mm ðmþ1Þ

III 0.0350 1.21 0.8814

IV 0.1004 1.48 0.8961

V 0.0486 1.14 0.9947

VI 0.0597 1.19 0.9961

constant in Eq. (11) Z 0:92. The discrete **dislocation** **plasticity** calculations do not predict

a linear scaling **of** d s with F max =S as required by Eq. (11) and predicted by **the** elastic finite

element calculations. In fact, over **the** range **of** **indentation** depths considered in Fig. 15b,

**the** calculations suggest that d s is relatively independent **of** F max =S.

As in experiments, **the** determination **of** S from F–d curves in **the** simulations tends to be

inaccurate. As a work-around, Oliver and Pharr (1992) suggest fitting a relation **of** **the**

form

F ¼ aðd d f Þ m , (13)

to **the** unloading curves and **the**n estimating **the** initial unloading stiffness as

S

dF

dd

d¼d max

¼ amðd max d f Þ m 1 . (14)

Here, d f is **the** residual **indentation** depth upon complete unloading while d max is **the**

**indentation** depth at which unloading commenced. We fit Eq. (13) to some **of** **the** discrete

**dislocation** **plasticity** predictions **of** **the** unloading curves using a least-squares fit. These fits

are included in Fig. 15a as dashed lines and **the** corresponding fitting parameters are listed

in Table 2 (along with **the** correlation coefficient R). As in **the** experimental observations

2300

ARTICLE IN PRESS

D.S. Balint et al. / J. Mech. Phys. Solids 54 (2006) 2281–2303

reported by Oliver and Pharr (1992), **the** predicted power-law exponents are in **the** range

m ¼ 1:1–1:4. The F max =S versus d s relation predicted by fitting Eq. (13) to **the** discrete

**dislocation** calculations is included in Fig. 15b with open symbols. The fitting procedure **of**

Oliver and Pharr (1992) also does not give results consistent with **the** elastic scaling relation

Eq. (11), although **the** agreement is better than obtained using **the** direct estimate **of** S

obtained from **the** unloading discrete **dislocation** calculations.

The discrepancy between Eq. (11) and **the** discrete **dislocation** predictions could arise

from: (i) material sink-in in **the**se calculations is not solely due to elastic deformations, i.e.

**the** **dislocation**s affect material sink-in and (ii) unloading is not purely elastic in **the** discrete

**dislocation** calculations.

In order to illustrate **the** occurrence **of** reverse **plasticity**, **the** evolution **of** **the** **dislocation**

density with **indentation** depth for **the** o ¼ 5 **indentation** **of** **the** h ¼ 50 mm film is plotted

in Fig. 16a. Here, **the** **dislocation** density is **the** number **of** **dislocation**s per unit area in a

region extending 25 mm on each side **of** **the** indenter tip and **the** 50 mm through **the** film

thickness. The data for **the** evolution **of** **the** **dislocation** density during unloading are also

included in Fig. 16a for **the** six unloading simulations performed. The figure clearly shows

that significant **dislocation** activity occurs during **the** initial unloading period with **the**

**dislocation** density increasing during unloading. This ‘‘reverse **plasticity**’’ is more

significant for unloading from **the** larger **indentation** loads and contributes to **the**

disagreement **of** **the** discrete **dislocation** predictions with Eq. (11). It is worth noting that

**the** two-dimensional discrete **dislocation**s calculations may overestimate **the** effect **of**

reverse **plasticity**. Three-dimensional discrete **dislocation**s simulations are needed in order

to ascertain whe**the**r or not **the** effect obtained here is an overestimate.

While **the** discrete **dislocation** predictions are not in agreement with Eq. (11), **the** main

aim **of** **the** Oliver and Pharr (1992) procedure is to estimate **the** actual contact length A.

20

15

8

7

6

S from simulation

S from fit to unloading data

ρ dis (µm -2 )

10

VI

A e (µm)

5

A e = A

4

3

5

0

0

(a)

I

0.1

II

V

IV

III

0.2

δ (µm)

0.3

0.4

(b)

2

1

0

0 1 2 3 4 5 6 7 8

A (µm)

Fig. 16. **Discrete** **dislocation** **plasticity** predictions for **the** **indentation** **of** **the** h ¼ 50 mm film **of** **the** reference

material by **the** o ¼ 5 indenter. (a) Predictions **of** **the** evolution **of** **the** **dislocation** density with **indentation** depth.

The evolution **of** **the** **dislocation** density for unloading from **the** six selected points marked in Fig. 15a are also

included. (b) A comparison between **the** estimated contact length A e with **the** actual contact length A.

Here an estimated contact length, A e , is calculated in two ways: (i) **the** unloading stiffness S

is estimated directly from **the** discrete **dislocation** calculations; and (ii) **the** value **of** S is

obtained from **the** fit Eq. (13). In both cases, **the** line labeled ‘‘elastic calculation’’ in

Fig. 15b is used to obtain d s for a given F max =S. This value **of** d s is **the**n used in Eq. (12) to

calculate **the** estimated contact length A e . A comparison between **the** estimated contact

length, A e , and **the** actual contact length, A, is shown in Fig. 16b for **the** o ¼ 5

**indentation** **of** **the** h ¼ 50 mm film with **the** reference crystal properties (no estimate based

on **the** fitting relation Eq. (13) is shown for **the** first two points because **the** unloading

calculations for **the**se were not continued to zero **indentation** pressure). In both cases, **the**

estimated contact length exceeds **the** actual contact length though **the** discrepancy is small

when **the** fit Eq. (13) is employed to determine S. At least in **the** cases considered here, **the**

Oliver and Pharr (1992) procedure using **the** power-law fit Eq. (13) toge**the**r with an elastic

**analysis** provides a good estimate **of** **the** actual contact area even though **the** initial

unloading stiffness is not accurately represented.

7. Conclusions

ARTICLE IN PRESS

D.S. Balint et al. / J. Mech. Phys. Solids 54 (2006) 2281–2303 2301

We have carried out plane strain analyses **of** **the** **indentation** **of** single crystal **films** by

rigid **wedge**-shaped indenters. While **the** computations are carried out within a small-strain

framework, contact is modeled by considering **the** deformed surface pr**of**ile **of** **the** **films**.

Films with thicknesses h **of** 2, 10 and 50 mm were analyzed. The crystals are initially

**dislocation**-free with **dislocation** nucleation occurring from Frank–Read sources **of** a

specified density, randomly distributed in **the** crystal. The discrete **dislocation** calculations

predict:

When **the** film thickness is sufficiently large relative to **the** **indentation** depth, **the**

**indentation** pressure decreases with increasing contact length. For sufficiently thick

**films**, with both **the** reference and low **dislocation** source density (LSD) crystal

properties, a size-independent **indentation** pressure is attained as **the** **indentation** depth

increases. This contact size-independent **indentation** pressure is in good agreement with

**the** prediction **of** conventional continuum crystal **plasticity** **the**ory. For small contact

depths, **the** **indentation** pressure with **the** LSD crystal properties is significantly greater

than with **the** reference crystal properties.

For **films** with h ¼ 2 mm, **the** **indentation** pressure initially decreases with increasing

contact length and **the**n increases with contact size when **the** plastic zone reaches **the**

rigid substrate. This occurs at an **indentation** depth **of** d=h 0:04 and 0.1 for **the** o ¼ 5

and 10 **wedge**s, respectively.

Over **the** range **of** **indentation** depths considered, material sink-in is predicted for **the** 10

and 50 mm **films**, while material pile-up occurs for **the** h ¼ 2 mm film when **the** plastic

zone reaches **the** substrate. With sink-in **the** actual **indentation** pressure is typically

greater than **the** nominal **indentation** pressure, but this is reversed for **the** h ¼ 2 mm film

when pile-up occurs.

The nominal **indentation** pressure versus depth relation can be described by power-law

relation in one **of** two ways: (i) with a power-law exponent **of** 0:5 as in Nix and Gao

(1998); or (ii) with a best-fit power-law exponent ranging between 0.6 and 0.7. With **the**

best-fit power-law exponent, **the** parameters in **the** relation have values on **the** order **of**

physically identifiable quantities—**the** continuum crystal **plasticity** limit for **the**

2302

ARTICLE IN PRESS

D.S. Balint et al. / J. Mech. Phys. Solids 54 (2006) 2281–2303

**indentation** pressure and **the** **dislocation** source and obstacle spacings for **the**

characteristic length. The value **of** **the** characteristic length also increases with

increasing **wedge** angle.

Over **the** range **of** parameters considered in **the** plane strain analyses here, nei**the**r **the**

initial unloading slope nor **the** amount **of** material sink-in are accurately modeled using

estimates based on a conventional continuum **analysis**. However, **the** actual (but not

accounting for any effect **of** surface roughness) contact area is well-modeled by an

elastic unloading **analysis** in conjunction with **the** fitting procedure **of** Oliver and Pharr

(1992).

Finally, we note that at a sufficiently small scale, **dislocation** nucleation from surfaces, in

particular from surface steps, as presumed in **the** model **of** Hurtado and Kim (1999a, b)

may play a prominent role. At present, no criterion has been developed for surface-step

**dislocation** nucleation that is appropriate for use in a discrete **dislocation** **plasticity**

formulation. The development **of** such a criterion and an **analysis** accounting for **the**

possibility **of** both surface and bulk **dislocation** nucleation would be a significant

additional step.

Acknowledgments

D.S.B. and V.S.D. acknowledge support from **the** Leverhulme Trust, UK. A.N. is

pleased to acknowledge support from **the** Materials Research Science and Engineering

Center at Brown University (NSF Grant DMR-0520651).

References

Abu Al-Rub, R.K., Voyiadjis, G.Z., 2004. Analytical and experimental determination **of** **the** material intrinsic

length scale **of** strain gradient **plasticity** **the**ory from micro- and nano-**indentation** experiments. Int. J.

Plasticity 20, 1139–1182.

Begley, M.R., Hutchinson, J.W., 1998. The mechanics **of** size-dependent **indentation**. J. Mech. Phys. Solids 46,

2049–2068.

Benzerga, A.A., Bréchet, Y., Needleman, A., der Giessen, E.V., 2004. Incorporating three-dimensional

mechanisms into two-dimensional **dislocation** dynamics. Modelling Simulation Mater. Sci. Eng. 12, 159–196.

Bhattacharya, A.K., Nix, W.D., 1988. Analysis **of** elastic and plastic deformation associated with **indentation**

testing **of** thin **films** on substrates. Int. J. Solids Struct. 24, 1287–1298.

Bouvier, S., Needleman, A., 2006. Effect **of** **the** number and orientation **of** active slip systems on plane strain

single crystal **indentation**. Modelling Simulation Mater. Sci. Eng., submitted for publication.

Cheng, C.M., Cheng, Y.T., 1997. On **the** initial unloading slope in **indentation** **of** elastic–plastic solids by an

indenter with an axisymmetric smooth pr**of**ile. Appl. Phys. Lett. 71, 2623–2625.

Cleveringa, H.H.M., Van der Giessen, E., Needleman, A., 1999. A discrete **dislocation** **analysis** **of** bending. Int. J.

Plasticity 15, 837–868.

Deshpande, V.S., Needleman, A., Van der Giessen, E., 2005. Plasticity size effects in tension and compression **of**

single crystals. J. Mech. Phys. Solids 53, 2661–2691.

Fivel, M.C., Robertson, C.F., Canova, G.R., Boulanger, L., 1998. Three-dimensional modeling **of** indent-induced

plastic zone at a mesoscale. Acta Mater. 46, 6183–6194.

Fleck, N.A., Hutchinson, J.W., 1997. Strain gradient **plasticity**. In: Hutchinson, J.W., Wu, T.Y. (Eds.), Advances

in Applied Mechanics, vol. 33. Academic Press, New York, p. 296.

Freund, L.B., 1994. The mechanics **of** **dislocation**s in strained-layer semiconductor-materials. Adv. Appl. Mech.

30, 1–66.

Freund, L.B., Suresh, S., 2004. Thin Film Materials: Stress, Defect Formation and Surface Evolution. Cambridge

University Press, Cambridge, UK.

ARTICLE IN PRESS

D.S. Balint et al. / J. Mech. Phys. Solids 54 (2006) 2281–2303 2303

Gerberich, W.W., Tymiak, N.I., Grunlan, J.C., Horstemeyer, M.F., Baskes, M.I., 2002. Interpretations **of**

**indentation** size effects. J. Appl. Mech. 69, 433–442.

Gouldstone, A., Koh, H.J., Zeng, K.Y., Giannakopoulos, A.E., Suresh, S., 2000. **Discrete** and continuous

deformation during **indentation** **of** thin **films**. Acta Mater. 48, 2277–2295.

Han, S.M., Saha, R., Nix, W.D., 2006. Determining hardness **of** thin **films** in elastically mismatched film-onsubstrate

systems using nano**indentation**. Acta Mater. 54, 1571–1581.

Horstemeyer, M.F., Baskes, M.I., Plimpton, S.J., 2001. Computational nanoscale **plasticity** simulations using

embedded atom potentials. Theor. Appl. Fract. Mech. 37, 49–98.

Huang, Y., Zhang, F., Hwang, K.C., Nix, W.D., Pharr, G.M., Feng, G., 2006. A model **of** size effects in nano**indentation**.

J. Mech. Phys. Solids 54, 1668–1686.

Hurtado, J.A., Kim, K.-S., 1999a. Scale effects in friction **of** single-asperity contacts I. From concurrent slip to

single-**dislocation**-assisted slip. Proc. R. Soc. London A 455, 3363–3384.

Hurtado, J.A., Kim, K.-S., 1999b. Scale effects in friction **of** single-asperity contacts II. Multiple-**dislocation**cooperated

slip. Proc. R. Soc. London A 455, 3385–3400.

Johnson, K.L., 1970. The correlation **of** **indentation** experiments. J. Mech. Phys. Solids 18, 115–126.

Kreuzer, H.G.M., Pippan, R., 2004. **Discrete** **dislocation** simulation **of** nano**indentation**. Comput. Mech. 33,

292–298.

Kreuzer, H.G.M., Pippan, R., 2005. **Discrete** **dislocation** simulation **of** nano**indentation**: **the** effect **of** statistically

distributed **dislocation**s. Mater. Sci. Eng. A 400–401, 460–462.

Kysar, J.W., Gan, Y.X., Morse, T.L., Chen, X., Huh, W.T., 2005. Indentation **of** face-centered cubic crystals:

measurement **of** lattice rotation and geometrically necessary **dislocation** density, in preparation.

Lou, J., Shrotriya, P., Buchheit, T., Yang, D., Soboyejo, W.O., 2003. Nano**indentation** study **of** **plasticity** length

scale effects in LIGA Ni microelectromechanical systems structures. J. Mater. Res. 18, 719–728.

Ma, Q., Clarke, D.R., 1995. Size dependent hardness **of** silver single crystals. J. Mater. Res. 10, 853–863.

Miller, R.E., Shilkrot, L.E., Curtin, W.A., 2004. A coupled atomistics and discrete **dislocation** **plasticity**

simulation **of** nano**indentation** into single crystal thin **films**. Acta Mater. 52, 271–284.

Nix, W.D., Gao, H., 1998. Indentation size effects in crystalline materials: a law for strain gradient **plasticity**.

J. Mech. Phys. Solids 43, 411–423.

Oliver, W.C., Pharr, G.M., 1992. An improved technique for determining hardness and elastic-modulus using

load and displacement sensing **indentation** experiments. J. Mater. Res. 7, 1564–1583.

Oliver, W.C., Pharr, G.M., 2004. Measurement **of** hardness and elastic modulus by instrumented **indentation**:

advances in understanding and refinements to methodology. J. Mater. Res. 19, 3–20.

Polonsky, I.A., Keer, L.M., 1996. Simulation **of** microscopic elastic–plastic contacts by using discrete **dislocation**s.

Proc. R. Soc. London A 452, 2173–2194.

Poole, W.J., Ashby, M.F., Fleck, N.A., 1996. Micro-hardness **of** annealed and work-hardened copper

polycrystals. Scr. Mater. 34, 559–564.

Qu, S., Huang, Y., Pharr, G.M., Hwang, K.C., 2006. The **indentation** size effect in **the** spherical **indentation** **of**

iridium: a study via **the** conventional **the**ory **of** mechanism-based strain gradient **plasticity**. Int. J. Plasticity 22,

1265–1286.

Rice, J.R., 1987. Tensile crack tip fields in elastic ideally plastic crystals. Mech. Mater. 6, 317–335.

Saha, R., Xue, Z., Huang, Y., Nix, W.D., 2001. Indentation **of** a s**of**t metal film on a hard substrate: strain

gradient hardening effects. J. Mech. Phys. Solids 49, 1997–2014.

Swadener, J.G., George, E.P., Pharr, G.M., 2002. The correlation **of** **the** **indentation** size effect measured with

indenters **of** various shapes. J. Mech. Phys. Solids 50, 681–694.

Tabor, D., 1951. Hardness **of** Metals. Clarendon Press, Oxford, UK.

Van der Giessen, E., Needleman, A., 1995. **Discrete** **dislocation** **plasticity**: a simple planar model. Modelling

Simulation Mater. Sci. Eng. 3, 689–735.

Wei, Y., Hutchinson, J.W., 2003. Hardness trends in micron scale **indentation**. J. Mech. Phys. Solids 51,

2037–2056.

Widjaja, A., Van der Giessen, E., Needleman, A., 2005. **Discrete** **dislocation** modelling **of** submicron **indentation**.

Mater. Sci. Eng. A 400–401, 456–459.

Widjaja, A., Needleman, A., Deshpande, V.S., VanderGiessen, E., 2006. On contact and size effects in discrete

**dislocation** modelling **of** **wedge** **indentation**, submitted for publication.

Zhu, T., Li, J., Van Vliet, K.J., Yip, S., Suresh, S., 2003. Simulation **of** nano**indentation** via interatomic potential

finite element method. Comput. Fluid Solid Mech. 1–2, 795–799.